Journal of Hazardous Materials 283 (2015) 164–170
Contents lists available at ScienceDirect
Journal of Hazardous Materials journal homepage: www.elsevier.com/locate/jhazmat
Conducting polypyrrole ﬁlms as a potential tool for electrochemical treatment of azo dyes in textile wastewaters Md. Mominul Haque a , Warren T. Smith b , Danny K.Y. Wong a,∗ a b
Department of Chemistry and Biomolecular Sciences, Macquarie University, Sydney, NSW 2109, Australia Samadha Paciﬁca Pty Ltd, Woonona, NSW 2517, Australia
h i g h l i g h t s • • • •
Anion exchange property of polypyrrole ﬁlms exploited in developing a treatment method for Acid Red 1. An environmentally friendly treatment method for Acid Red 1 without generating any toxic by-products. Acid Red 1 is anodically entrapped and cathodically liberated at polypyrrole ﬁlms. Analytical characteristics of Acid Red 1-entrapped polypyrrole ﬁlms.
a r t i c l e
i n f o
Article history: Received 15 May 2014 Received in revised form 17 July 2014 Accepted 18 July 2014 Available online 29 July 2014 Keywords: Electrochemical treatment Dye entrapment–liberation Polypyrrole ﬁlms Acid Red 1 Environmentally friendly treatment
a b s t r a c t In this paper, we demonstrate conducting polypyrrole ﬁlms as a potential green technology for electrochemical treatment of azo dyes in wastewaters using Acid Red 1 as a model analyte. These ﬁlms were synthesised by anodically polymerising pyrrole in the presence of Acid Red 1 as a supporting electrolyte. In this way, the anionic Acid Red 1 is electrostatically attracted to the cationic polypyrrole backbone formed to maintain electroneutrality, and is thus entrapped in the ﬁlm. These Acid Red 1-entrapped polypyrrole ﬁlms were characterised by electrochemical, microscopic and spectroscopic techniques. Based on a two-level factorial design, the solution pH, Acid Red 1 concentration and polymerisation duration were identiﬁed as signiﬁcant parameters affecting the entrapment efﬁciency. The entrapment process will potentially aid in decolourising Acid Red 1-containing wastewaters. Similarly, in a cathodic process, electrons are supplied to neutralise the polypyrrole backbone, liberating Acid Red 1 into a solution. In this work, following an entrapment duration of 480 min in 2000 mg L−1 Acid Red 1, we estimated 21% of the dye was liberated after a reduction period of 240 min. This allows the recovery of Acid Red 1 for recycling purposes. A distinctive advantage of this electrochemical Acid Red 1 treatment, compared to many other techniques, is that no known toxic by-products are generated in the treatment. Therefore, conducting polypyrrole ﬁlms can potentially be applied as an environmentally friendly treatment method for textile efﬂuents. © 2014 Elsevier B.V. All rights reserved.
1. Introduction Azo dyes are among the most widely used groups of dyes in textile applications . This is mainly due to their cost effectiveness, ease of synthesis and intense colouring properties. Owing to their high solubility in water , potential carcinogenicity , intense colours  and non-reactive nature , azo dyes are known to exhibit various adverse effects upon aquatic ﬂora and fauna . This becomes an even more severe issue in environments where
∗ Corresponding author. Tel.: +61 2 9850 8300; fax: +61 2 9850 8313. E-mail address: [email protected]
(D.K.Y. Wong). http://dx.doi.org/10.1016/j.jhazmat.2014.07.038 0304-3894/© 2014 Elsevier B.V. All rights reserved.
existence of dyes persists for a long period of time. Their intense colours in an aqueous system also inevitably decrease the amount of sunlight penetration, causing a reduction in the rate of photosynthesis, which in turn affects various life forms in the water body . Several treatment methods for azo dyes have hitherto been reported. These include microbial degradation , adsorbents (e.g. active carbon) [8,9], sacriﬁcial iron electrodes , electrolysis [11,12], electrocoagulation [13,14], ion-pair extraction , Fenton’s process and other advanced electrochemical oxidation processes [16,17]. However, there are severe limitations associated with these methods. For example, there are disposal problems concerning spent carbon in using active carbon as an adsorbent
Md.M. Haque et al. / Journal of Hazardous Materials 283 (2015) 164–170
Fig. 1. Structure of the azo dye, Acid Red 1.
ﬁlms are selective towards the original counter anion used, and the size of the counter anion controls the microstructure and porosity of the ﬁlms. The relation between the porosity of the membrane and afﬁnity for certain anions suggests a memory effect in terms of selectivity of the polypyrrole ﬁlms . In other words, after entrapping a particular anion in the polypyrrole ﬁlm, speciﬁc channels for the anion are formed. This behaviour was used to explain the polypyrrole–anion ﬁlms selectivity towards the targeted anion. In this paper, we have demonstrated the application of polypyrrole as a potential tool for treatment of azo dyes in textile efﬂuents, using Acid Red 1 as a model dye. Initially, pyrrole was electrochemically oxidised in the presence of Acid Red 1 as a counter ion to synthesise an Acid Red 1-entrapped polypyrrole ﬁlm (denoted as a polypyrrole–Acid Red 1 ﬁlm). The ﬁlms obtained were then characterised by electrochemistry, scanning electron microscopy and spectrophotometry. Experimental conditions for Acid Red 1 entrapment in polypyrrole ﬁlms were also optimised using a two-factorial experimental design. Finally, we have evaluated the liberation efﬁciency of Acid Red 1 after electrochemically reducing polypyrrole–Acid Red 1 ﬁlms. 2. Experimental
[18,19]. Fenton’s process also generates appreciable quantity of ferric hydroxide sludge that requires further treatment before proper disposal . Meanwhile, microbial degradation-based biological treatments are very slow processes due to their limitation in decomposing macromolecular dyes. In addition, the majority of these dyes are chemically stable and resistant to microbiological attack as a result of low degradation efﬁciency . Notably, chemical and electrochemical oxidation treatments often produce toxic by-products during operation. As an example, the electrochemical oxidation of the azo dyes, azobenzene, p-methyl red, methyl orange, Orange G and Sunset Yellow FCF will produce 1,4-benzoquinone, pyrocatechol, 4-nitrocatechol, 1,3,5-trihydroxynitrobenzene, p-nitrophenol, hydrazine, aromatic amines, respectively, which are carcinogenic and more toxic than the original dye molecules [15,22,23]. Therefore, there is a need for developing alternative treatments that are effective and environmentally friendly in removing dyes from textile efﬂuents. Among the azo dyes, Acid Red 1 (5-(acetylamino)-4-hydroxy3-[[4-(phenylamino)phenyl]azo]-2,7-naphthalenedisulfonic acid disodium salt), the structure of which is shown in Fig. 1, has been classiﬁed as a non-biodegradable dye by the Environment Protection Agency . This is a potential environmental concern, not only that it generates aesthetical problems associated with decolourisation of the water body, but there are also evidences for the carcinogenic effect of its degradation products in anaerobic conditions [25–27]. In the ﬁeld of conducting polymers, polypyrrole has received a lot of recognition in the last decade due to its high conductivity (up to 2000 S cm−1 )  and mechanical and thermal stability [29,30]. As shown in Fig. 2 below, the synthesis of polypyrrole usually involves electrochemical oxidation of its monomer, pyrrole, to yield a polymeric chain with a positive backbone. In order to neutralise this charge, a counter anion, for example, that of ptoluene sulfonate (pTS− ), is entrapped in the backbone structure. The polypyrrole–pTS− ﬁlm has long been known to exhibit conductivity as high as 160 S cm−1 . Many studies have shown that this entrapment process is electrochemically reversible [30,32], enabling polypyrrole to act as an anion exchanger, depending upon the mobility of the entrapped counter anion . Clearly, mobile anions can also be easily liberated from the polymeric ﬁlm, as shown in Fig. 2. In this respect, several researchers have described the transport of small organic molecules, for example, aza crown ether and tosylate, across polypyrrole by an anion exchanging mechanism [34–36]. These reports also found that the polypyrrole
2.1. Materials Acid Red 1 and pyrrole were purchased from Sigma–Aldrich (Sydney, Australia). Pyrrole was always doubly vacuum distilled at 130 ◦ C and then stored in a light protected bottle at 4 ◦ C until required for use. All aqueous solutions were prepared using deionised water puriﬁed by a Milli Q water system (Millipore). High purity nitrogen gas (BOC) was used to purge all analyte solutions for 10 min at the beginning of an experiment. 2.2. Apparatus All voltammetric studies were performed using a MacLab/200 System operated by EChem and Chart software (eDaq Pty Ltd, Sydney, Australia). A 50-mL vial was used as an electrochemical cell accommodating a three-electrode system. A stainless steel plate (3 cm × 1.5 cm) and a same-sized stainless steel mesh (both manufactured by Macquarie Engineering and Technical Services, Macquarie University) were used as a working electrode and a counter electrode, respectively. All potentials were recorded relative to a Ag|AgCl (in 3 mol L−1 KCl) reference electrode. UV–visible spectroscopy was performed using a Bio Spectrophotometer (Eppendorf, Australia). The morphology of the polypyrrole–Acid Red 1 ﬁlms were analysed by a JEOL JSM-6480 scanning electron microscope operated with an accelerating voltage of 10 kV. Conductivity measurements were performed using a locally constructed four-point probe. 2.3. Electropolymerisation of polypyrrole–Acid Red 1 ﬁlms Each polypyrrole–Acid Red 1 ﬁlm was galvanostatically polymerised on a stainless steel working electrode in the presence of 0.2 mol L−1 pyrrole and Acid Red 1 of concentration 60–2000 mg L−1 for a duration from 20 to 480 min. The polypyrrole–Acid Red 1 ﬁlm was carefully removed from the electrode before being used in further characterisation experiments. The remaining electrolyte solution in the cell was also used in the entrapment analysis. 2.4. X-ray diffraction analysis X-ray diffraction (XRD) analysis was conducted to identify the crystalline phase of the polypyrrole–Acid Red 1 ﬁlm samples. In these experiments, polypyrrole–Acid Red 1 ﬁlms were placed on
Md.M. Haque et al. / Journal of Hazardous Materials 283 (2015) 164–170
Fig. 2. Schematic diagram for pyrrole oxidation and polypyrrole reduction in the presence of the counter ion, pTS− .
a Si wafer (1 1 1) before being analysed on an X’Pert Pro MPD X-ray diffractometer (Philips® , Netherlands). A voltage of 40 kV and an anode current of 40 mA were applied. A Cu K␣ radiation ( = 0.15405 nm) was used in a continuous scanning mode with 0.02 step size and 0.5 s set time for collecting the data in a 2 scan range of 4◦ –20◦ . 2.5. Fourier transform infrared spectroscopic analysis Fourier transform infrared spectroscopy (FTIR) was used to analyse polypyrrole ﬁlms. The spectra were obtained over 16 scans covering the 4000–650 cm−1 wave number range at 4 cm−1 resolution and at 25 ◦ C using a Thermo Scientiﬁc Nicolet iS10 FTIR spectrometer. 2.6. Entrapment and liberation experiments All experiments were carried out at room temperature. At the end of each polymerisation experiment, the pyrrole and Acid Red 1 mixture was analysed by UV–visible spectrophotometry at 530 nm to estimate the ﬁnal concentration of Acid Red 1. The percentage of Acid Red 1 entrapped in a polypyrrole ﬁlm was then evaluated based on the difference (in mg L−1 ) between the initial concentration (Cinitial ) and the ﬁnal concentration (Cﬁnal ) of Acid Red 1. Taking into consideration the total solution volume (V in L) and the initial mass of the polypyrrole ﬁlm (m in g), the mass of Acid Red 1 per mass of polypyrrole ﬁlm (q in mg g−1 ) was then evaluated according to Eq. (1). q=
Cﬁnal − Cinitial m
3. Results and discussion 3.1. Electrochemical characterisation of polypyrrole–Acid Red 1 ﬁlms In this work, we are exploiting the anion entrapping–liberating mechanism at a polypyrrole ﬁlm to develop a feasible treatment method for dye molecules in textile efﬂuents. We have chosen the azo dye, Acid Red 1, as a model analyte in this pilot study. Initially, cyclic voltammetry of 0.2 mol L−1 pyrrole was conducted at a stainless steel electrode in the presence of 1500 mg L−1 (∼0.0018 mol L−1 ) Acid Red 1 as a supporting electrolyte. We have used a stainless steel electrode in this work solely because it is an economical material for construction of bigger-size electrodes when necessary. Trace (a) in Fig. 3 shows the cyclic voltammogram obtained. Here, an oxidation peak at 0.76 V was observed as the potential was scanned from −1.0 V to 1.0 V, and a reduction peak at −0.64 V as the potential was scanned backward. The former peak was attributed to the oxidation of pyrrole to form polypyrrole with
In our experiments, Acid Red 1 was cathodically liberated from dye-entrapped polypyrrole ﬁlms placed in a 0.1 M KNO3 supporting electrolyte by applying −0.80 V (versus Ag|AgCl) for different duration. The resultant solution was again spectrophotometrically analysed at 530 nm to determine the liberation efﬁciency according to Eq. (2). %Liberation =
ﬁnal × 100 Cﬁnal − Cinitial
2.7. Optimisation experiments A two-factorial design was used to identify the signiﬁcant factors in Acid Red 1 entrapment in polypyrrole ﬁlms. These factors included solution pH, adsorption time, Acid Red 1 concentration and pyrrole concentration.
Fig. 3. Cyclic voltammetry of 0.2 M pyrrole at a stainless steel electrode in 1500 mg L−1 Acid Red 1 as supporting electrolyte; scan rate 100 mV s−1 .
Md.M. Haque et al. / Journal of Hazardous Materials 283 (2015) 164–170
Fig. 4. Scanning electron micrograph of the electrolyte-facing surface of a polypyrrole–Acid Red 1 ﬁlm.
a positively charged backbone with entrapped Acid Red 1 anion, while the latter peak arose from the reduction of polypyrrole to form an uncharged, Acid Red 1 liberated ﬁlm. The voltammogram shown in trace (a) is comparable to that of a very broad oxidation peak between 0.1 and 0.6 V and a sharper reduction peak at −0.7 V (versus Ag|AgCl) for the formation of polypyrrole ﬁlms in the presence of 1.0 M KNO3 . In contrast, trace (b) shows a featureless cyclic voltammogram obtained in the Acid Red 1 supporting electrolyte without any pyrrole. Notably, Wang et al.  also observed no Acid Red 1 oxidation/reduction peaks at a glassy carbon electrode in 0.1 mol L−1 Na2 SO4 solution between −1.0 V and 1.0 V. Based on trace (a), an oxidation potential of 0.88 V, which is more positive than the oxidation peak potential, and a reduction potential of −0.80 V, which is more negative than the reduction peak potential, were selected to be the respective potential for entrapment and liberation of Acid Red 1 at polypyrrole ﬁlms in our studies below. In our work, we have also measured the conductivity of polypyrrole–Acid Red 1 ﬁlms formed in 0.2 M pyrrole and 1500 mg L−1 of Acid Red 1 solution to be 18 S cm−1 (with a standard deviation of 1.2 S cm−1 ; N = 7). Our results are comparable to 2–18 S cm−1 obtained by Wang et al.  using polypyrrole ﬁlms doped with different sulfonic acids. Clearly Acid Red 1 is bulkier and less mobile than smaller aromatic sulfonates such as pTS− , and this leads to less well ordered polypyrrole ﬁlms of lower conductivity. 3.2. Scanning electron microscopic study of polypyrrole–Acid Red 1 ﬁlms Scanning electron microscopy was employed to study the surface morphology of the polypyrrole–Acid Red 1 ﬁlms. Fig. 4 shows typical ‘cauliﬂower’ like structures on the electrolyte-facing surface of such ﬁlms, similar to those previously observed at polypyrrole ﬁlms polymerised in the presence of p-toluene sulfonic acid . Notably, the ﬁlm surface is not ﬂat, but consists of a series of peaks and valleys with considerable surface roughness associated with a high degree of ﬁlm porosity. 3.3. FTIR of polypyrrole–Acid Red 1 ﬁlms Next, the polypyrrole–Acid Red 1 ﬁlms was analysed by FTIR. The spectra of a polypyrrole–Acid Red 1 ﬁlm and Acid Red 1 alone are shown in Fig. 5. The FTIR spectrum of a polypyrrole–Acid Red 1
Fig. 5. FTIR spectra of (a) a polypyrrole–Acid Red 1 ﬁlm and (b) Acid Red 1 alone.
ﬁlm in Fig. 5(a) shows three groups of weak bands at (1) ∼1660, 1490 and 1410 cm−1 , (2) ∼1050 cm−1 , (3) ∼980 and 898 cm−1 . Similar results were observed by Zhang et al.  and they have assigned these three groups of bands to ring stretching, N H bending of polypyrrole, in-plane and out-of-plane C H bending, respectively. In addition, according to Zhang et al.  and Li et al.  the absorption peaks at 898, 1256 cm−1 indicate the coupling of S O with the stretching vibration of the pyrrole ring, and that at 2600 cm−1 corresponds to the stretching vibration mode of methylene groups in the long alkyl chains of Acid Red 1. In comparison, the FTIR spectrum of Acid Red 1 alone in Fig. 5(b) shows characteristic absorption bands at 750, 1256 cm−1 corresponding to the strong stretching vibration of S O group and the peak at 1750 cm−1 corresponding to C O stretching of Acid Red 1. A broad and intense peak at 3450 cm−1 arose from the OH stretching band of Acid Red 1. Therefore, the presence of these peaks in Fig. 5(a) provides further evidence of Acid Red 1 entrapment in polypyrrole. 3.4. XRD analysis of polypyrrole–Acid Red 1 ﬁlms In this experiment, XRD analysis was carried out as a complementary technique for examining the entrapment of Acid Red 1 in polypyrrole ﬁlms. Previously, Ferreira et al.  analysed XRD patterns of polypyrrole synthesised with the dyes Remazol Black B and Dianix Red. In their work, they proposed a structure consisting of a dye sandwiched between two polypyrrole chains separated by a perpendicular distance termed “d-spacing”, which can be evaluated based on Bragg’s law  in Eq. (3), = 2d sin
where denotes the Cu K␣ radiation wavelength ( = 0.15405 nm in our work) and sin is derived from the lowest 2 signal in a diffraction pattern. The diffraction patterns of a polypyrrole–Acid Red 1 ﬁlm, depicted in Fig. 6(a), shows a sharp peak at the lowest 2 diffraction angle of 8.62. For comparison, the XRD patterns of a polypyrrole–NO3 − ﬁlm alone, shown in Fig. 6(b), do not reveal any distinct peaks. The result of Acid Red 1 alone is displayed in Fig. 6(c), which also shows a 2 peak at 8.62, supporting the origin of this
where sp is a pooled standard deviation,
m (degrees of freedom × variance) i=1 m degrees of freedom i=1
and m is the number of experimental conditions (m = 16 in this work), nF is the number of experimental replications (nF = 32). When the absolute value of tE is larger than the tabulated t-value
t*(16) = 2.12
31.13 6.16 9.72 24.50 873.62 2670.34 1225.13 2538.28 123.56 59.08 65.90 107.90 2051.20 3862.33 2346.13 3532.20 32.22 6.27 38.96 8.00 480.60 450.46 490.75 460.94 95.87 65.58 98.44 92.52 600.56 520.93 660.75 540.53
+ − − + − + + − − + + − + − − + 2296.52 2366.82 4663.34 −70.3 −8.79 −0.71 − − + + + + − − + + − − − − + + 2350.74 2312.6 4663.34 38.13 4.77 0.39 − + − + + − + − + − + − − + − + 2261.38 2401.96 4663.34 −140.59 −17.57 −1.42 − + + − + − − + − + + − + − − + 2301.85 2361.49 4663.34 −59.63 −7.45 −0.6 + + + + − − − − − − − − + + + + 2428.19 2235.15 4663.34 193.05 24.13 1.95 + + − − + + − − − − + + − − + + 2371.77 2291.57 4663.34 80.2 10.03 0.81 + + − − − − + + + + − − − − + + 2362.89 2300.45 4663.34 62.43 7.8 0.63 + − + − + − + − − + − + − + − + 2262.06 2401.28 4663.34 −139.22 −17.4 −1.41 + − + − − + − + + − + − − + − + 2238.33 2425.01 4663.34 −186.69 −23.34 −1.89
X1X4 X1X3 X1X2 X4 X3
+ − − + + − − + + − − + + − − + 2321.22 2342.12 4663.34 −20.9 −2.61 −0.21 DF, degrees of freedom.
Effect √ 2sp / nF
Code X values
Table 2 Model matrix and the results of the 24 factorial design.
Initially, it is necessary to determine the optimum experimental conditions for Acid Red 1 entrapment in polypyrrole ﬁlms. In our work, we have used a two-level factorial design not only to identify the signiﬁcant factors and determine their optimal values, but also to study possible interactions among these factors . We have considered factors including solution pH (denoted as X1 ), pyrrole concentration (Cpyrrole ; X2 ), Acid Red 1 concentration (CAcid Red 1 ; X3 ) and polymerisation time (X4 ). Accordingly, a 24 factorial design for four factors (16 experiments in total) was adopted. Table 1 shows the experimental factors and their levels employed in the 24 factorial design. Based on earlier experimental results and practical operation conditions, a low (−) and a high (+) level were assigned to each factor. Following electropolymerisation under the conditions speciﬁed for each run, the percentage weight of Acid Red 1 adsorbed per weight of polypyrrole ﬁlm was evaluated using Eq. (1). Two replicate measurements were conducted at each condition and the average results obtained at different computation of effects and interactions (X1 X2 , X1 X3 , X1 X4 , X2 X3 , X2 X4 , X3 X4 , X1 X2 X3 , X1 X3 X4 , X2 X3 X4 , X1 X2 X3 X4 ) for a 24 factorial design are shown in Table 2. Also, in Table 2, the Effect row represents the average of the high (+) and the low (−) values of each experimental factor, while tE represents a signal-to-noise ratio calculated by the expression
3.5. Optimisation of entrapment parameters
− − − − − − − − + + + + + + + + 2675.16 1988.18 4663.34 686.98 85.87 6.95
peak in Fig. 6(a). Accordingly, a d-spacing of 10.3 A˚ was estimated from Eq. (3). This distance suggests that, Acid Red 1 is sandwiched between two polymer chains, and it may act as a bridge between the chains.
− − + + − − + + − − + + − − + + 2400.87 2262.47 4663.34 138.41 17.3 1.4
12 0.6 2000 480
− + − + − + − + − + − + − + − + 2165.2 2498.14 4663.34 −332.94 −41.62 −3.37
2 0.1 60 20
+ + + + + + + + + + + + + + + + 4663.34 0 4663.34 4663.34 291.46
X1 X2 X3 X4
1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 ˙(+) ˙(−) ˙(+) + ˙(−) ˙(+) − ˙(−) Effect tE
Solution pH Cpyrrole /mol L−1 CAcid Red 1 /mg L−1 Time/min
1 2 3 4
High level (+)
Low level (−)
Table 1 Experimental factors and their levels employed in a 24 factorial design.
− − − − + + + + − − − − + + + + 4205.5 457.84 4663.34 3747.67 468.46 37.93
Variance Average dye entrapped/mg g−1 X1X2X3X4
Fig. 6. XRD patterns of (a) polypyrrole–Acid Red 1, (b) polypyrrole–NO3 − and (c) Acid Red 1.
1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1
Md.M. Haque et al. / Journal of Hazardous Materials 283 (2015) 164–170 DF
Md.M. Haque et al. / Journal of Hazardous Materials 283 (2015) 164–170
Fig. 8. Liberated Acid Red 1 from dye entrapped polypyrrole ﬁlms at various initial dye concentrations after different time interval.
Fig. 7. Effect of (a) pH, (b) polymerisation time and (c) Acid Red 1 concentration on Acid Red 1 entrapment in polypyrrole ﬁlms.
(denoted by t*) at the 95% conﬁdence level, the effect of a particular factor or interaction between factors is considered signiﬁcant. Accordingly, the results in Table 2 reveal that X1 , X3 and X4 are statistically signiﬁcant and X2 is not signiﬁcant. However, the results also show that none of the interactions is signiﬁcant. In this way, a prediction equation for our system can be written as: Y = 291.46 −
= 291.46 − 20.81X1 + 234.23X3 + 42.94X4
3.5.1. Effect of solution pH on Acid Red 1 entrapment at polypyrrole ﬁlms The pH of the Acid Red 1 solutions is one of the important factors inﬂuencing the entrapment process. The effect of the initial dye solution pH on Acid Red 1 entrapment efﬁciency at polypyrrole was studied between pH 2 and 12 and the results are shown in Fig. 7(a). A 480-min duration was allowed to entrap Acid Red 1 at different solution pH. In general, more Acid Red 1 was entrapped at polypyrrole ﬁlms in the pH 2–4 range and a maximum was observed at approximately pH 4. However, this entrapment efﬁciency of Acid Red 1 then decreased with higher solution pH. Previously, pyrrole was reported to be readily oxidised forming thick, smooth and conducting polypyrrole ﬁlms in acidic media and almost insulating ﬁlms under neutral conditions . However, no ﬁlm formation was observed in alkaline media owing to an inhibited oxidation of pyrrole . In this work, we observed that thin, fragile polypyrrole ﬁlms were formed in neutral and alkaline media, which did not favour efﬁcient entrapment of Acid Red 1.
3.5.2. Effect of initial Acid Red 1 concentration and polymerisation time on entrapment Entrapment of Acid Red 1 is also affected by the initial Acid Red 1 concentration and polymerisation time of polypyrrole. Fig. 7(b) shows the extent of Acid Red 1 entrapped at polypyrrole ﬁlms with increasing polymerisation time at various initial dye concentrations. Notably, when the initial Acid Red 1 concentration was increased from 60 to 2000 mg L−1 (∼0.002 mol L−1 –0.078 mol L−1 ), the extent of Acid Red 1 entrapped after 480 min increased from ∼51 to 690 mg g−1 . This is clearly attributed to an increased driving force arising from the concentration gradient with the higher initial dye concentration. However, over the same Acid Red 1 concentration range, the relative percentage of entrapped Acid Red 1 at polypyrrole ﬁlms decreased from 68 to 44% (depicted in Fig. 7(c)). This is most likely due to a limited number of active adsorption sites on polypyrrole ﬁlms, which were saturated at a particular concentration . Fig. 7(c) also shows that equilibrium was attained at an initial dye concentration of 1500 mg L−1 with little change at 2000 mg L−1 . 3.6. Liberation of Acid Red 1 from polypyrrole ﬁlms A polypyrrole ﬁlm–electrolyte system involves the redox cou• • ple, polypyrrole+ /polypyrrole , where polypyrrole+ is the radical cationic species and polypyrrole is the neutral species. • During oxidation, polypyrrole+ will electrostatically attract the anionic Acid Red 1 at the polypyrrole matrix so as to maintain electroneutrality. Similarly, during reduction, electrons are supplied and polypyrrole becomes neutral, leading to the liberation of Acid Red 1 from the polypyrrole ﬁlm to the solution. Indeed, this particular feature distinguishes the potential treatment method of textile efﬂuents using polypyrrole ﬁlms from many others reported in literature. In this way, Acid Red 1 itself can be recovered in the process. In this work, using UV–visible spectrophotometry, we have measured the concentration of the liberated Acid Red 1 in 0.1 mol L−1 KNO3 after applying a reduction potential of −0.80 V for a deﬁned period. This study was conducted on polypyrrole ﬁlms prepared with increasing Acid Red 1 concentrations from 60 to 2000 mg L−1 . The results obtained are shown in Fig. 8. In general, the concentration of Acid Red 1 liberated increased as the initial Acid Red 1 concentration was increased. However, no signiﬁcant increase in concentration of liberated Acid Red 1 was observed after prolonging the reduction process beyond 180 min. This is most likely because Acid Red 1 entrapped deep in the multilayered ﬁlm matrix on the stainless steel electrode would be unable to diffuse out from the ﬁlm interfaces. Consequently, a low recovery rate was observed. In this experiment, in the presence of an initial Acid Red 1 concentration of 2000 mg L−1 , a maximum liberation rate of 21%
Md.M. Haque et al. / Journal of Hazardous Materials 283 (2015) 164–170
was estimated following a reduction period of 240 min. Improvement on the liberation rate requires further work that involves, for example, development of polypyrrole ﬁlms with high porosity, polypyrrole–nanomaterial composite ﬁlms. 4. Conclusion In this study, we have exploited the anion entrapping–liberating property of conducting polypyrrole ﬁlms to develop a green treatment method for the model azo dye, Acid Red 1. By oxidising pyrrole at 0.88 V in the presence of Acid Red 1, the dye was readily entrapped in the polypyrrole ﬁlm. We then employed cyclic voltammetry, conductivity measurements, FTIR and X-ray diffraction to characterise these polypyrrole–Acid Red 1 ﬁlms and all results supported the presence of Acid Red 1 in polypyrrole ﬁlms synthesised in this way. In addition, based on a two-factorial design, the entrapment process was found to be dependent on pH, concentration of Acid Red 1 in solution and polymerisation time. The entrapped Acid Red 1 was then liberated from a polypyrrole ﬁlm by applying a reduction potential of −0.80 V. Our results suggest that electropolymerised conducting polypyrrole ﬁlms can be further developed as an effective and alternative material for treatment of dye efﬂuents. Further results on the performance of polypyrrole ﬁlms in the presence of multiple dyes will be reported in a separate publication. References  E.J. Ruiz, C. Arias, E. Brillas, A. Hernández-Ramírez, J. Peralta-Hernández, Mineralization of Acid Yellow 36azo dye by electro-Fenton and solar photoelectro-Fenton processes with a boron-doped diamond anode, Chemosphere 82 (2011) 495–501.  J. Riu, I. Schönsee, D. Barcelo, C. Rafols, Determination of sulphonated azo dyes in water and wastewater, TrAC: Trends Anal. Chem. 16 (1997) 405–419.  P. Li, G. Zhao, K. Zhao, J. Gao, T. Wu, An efﬁcient and energy saving approach to photocatalytic degradation of opaque high-chroma methylene blue wastewater by electrocatalytic pre-oxidation, Dyes Pigm. 92 (2012) 923–928.  P. Sarala, T. Venkatesha, Electrochemical degradation of p-aminobenzoic acid ␤-naphthol azo dye in alkaline solution, J. Environ. Chem. Ecotoxicol. 4 (2012) 116–123.  S.M. McClung, A.T. Lemley, Electrochemical treatment and HPLC analysis of wastewater containing acid dyes, Text. Chem. Color. 26 (1994) 17–22.  I.M. Banat, P. Nigam, D. Singh, R. Marchant, Microbial decolorization of textiledyecontaining efﬂuents: a review, Bioresour. Technol. 58 (1996) 217–227.  L. Ma, R. Zhuo, H. Liu, D. Yu, M. Jiang, X. Zhang, Y. Yang, Efﬁcient decolorization and detoxiﬁcation of the sulfonated azo dye Reactive Orange 16 and simulated textile wastewater containing Reactive Orange 16 by the white-rot fungus Ganoderma sp. En3 isolated from the forest of Tzu-chin Mountain in China, Biochem. Eng. J. 82 (2014) 1–9.  K.Y. Foo, B.H. Hameed, An overview of dye removal via activated carbon adsorption process, Desalin. Water Treat. 19 (2010) 255–274.  K. Dermentzis, Removal of nickel from electroplating rinse waters using electrostatic shielding electrodialysis/electrodeionization, J. Hazard. Mater. 173 (2010) 647–652.  M.Y. Mollah, S.R. Pathak, P.K. Patil, M. Vayuvegula, T.S. Agrawal, J.A. Gomes, M. Kesmez, D.L. Cocke, Treatment of orange II azo-dye by electrocoagulation (EC) technique in a continuous ﬂow cell using sacriﬁcial iron electrodes, J. Hazard. Mater. 109 (2004) 165–171.  M.J. Kupferle, A. Galal, P.L. Bishop, Electrolytic treatment of azo dye wastewaters: impact of matrix chloride content, J. Environ. Eng. 132 (2006) 514–518.  L. Xu, H. Zhao, S. Shi, G. Zhang, J. Ni, Electrolytic treatment of CI Acid Orange 7 in aqueous solution using a three-dimensional electrode reactor, Dyes Pigm. 77 (2008) 158–164.  A. Aleboyeh, N. Daneshvar, M. Kasiri, Optimization of CI Acid Red 14 azo dye removal by electrocoagulation batch process with response surface methodology, Chem. Eng. Process. 47 (2008) 827–832.  O. Can, M. Kobya, E. Demirbas, M. Bayramoglu, Treatment of the textile wastewater by combined electrocoagulation, Chemosphere 62 (2006) 181–187.  J.J. Gooding, R.G. Compton, C.M. Brennan, J.H. Atherton, The mechanism of the electro-reduction of some azo dyes, Electroanalysis 8 (1996) 519–523.  Y.-Y. Chu, W.-J. Wang, M. Wang, Anodic oxidation process for the degradation of 2,4-dichlorophenol in aqueous solution and the enhancement of biodegradability, J. Hazard. Mater. 180 (2010) 247–252.  H.S. El-Desoky, M.M. Ghoneim, N.M. Zidan, Decolorization and degradation of Ponceau S azo-dye in aqueous solutions by the electrochemical advanced Fenton oxidation, Desalination 264 (2010) 143–150.
 M.A. Hubbe, K.R. Beck, W.G. O’Neal, Y.C. Sharma, Cellulosic substrates for removal of pollutants from aqueous systems: a review. 2, Dyes BioResour. 7 (2012) 2592–2687.  J. Qu, Research progress of novel adsorption processes in water puriﬁcation: a review, J. Environ. Sci. 20 (2008) 1–13.  P. Chang, Y. Huang, C. Hsueh, M. Lu, G. Huang, Treatment of non-biodegradable wastewater by electro-Fenton method, Water Sci. Technol. 49 (2004) 213–218.  C. Pearce, J. Lloyd, J. Guthrie, The removal of colour from textile wastewater using whole bacterial cells: a review, Dyes Pigm. 58 (2003) 179–196.  E. Guivarch, S. Trevin, C. Lahitte, M.A. Oturan, Degradation of azo dyes in water by electro-Fenton process, Environ. Chem. Lett. 1 (2003) 38–44.  M.M. Tauber, G.M. Guebitz, A. Rehorek, Degradation of azo dyes by laccase and ultrasound treatment, Appl. Environ. Microbiol. 71 (2005) 2600–2607.  H.-Y. Shu, C.-R. Huang, M.-C. Chang, Decolorization of mono-azo dyes in wastewater by advanced oxidation process: a case study of acid red 1 and acid yellow 23, Chemosphere 29 (1994) 2597–2607.  K. Golka, S. Kopps, Z.W. Myslak, Carcinogenicity of azo colorants: inﬂuence of solubility and bioavailability, Toxicol. Lett. 151 (2004) 203–210.  F.P. Van der Zee, S. Villaverde, Combined anaerobic–aerobic treatment of azo dyes—a short review of bioreactor studies, Water Res. 39 (2005) 1425–1440.  H. Pinheiro, E. Touraud, O. Thomas, Aromatic amines from azo dye reduction: status review with emphasis on direct UV spectrophotometric detection in textile industry wastewaters, Dyes Pigm. 61 (2004) 121–139.  G. Qi, L. Huang, H. Wang, Highly conductive free standing polypyrrole ﬁlms prepared by freezing interfacial polymerization, Chem. Commun. 48 (2012) 8246–8248.  I.S. Chronakis, S. Grapenson, A. Jakob, Conductive polypyrrole nanoﬁbers via electrospinning: electrical and morphological properties, Polymer 47 (2006) 1597–1603.  S. Masubuchi, S. Kazama, K. Mizoguchi, F. Shimizu, K. Kume, R. Matsushita, T. Matsuyama, The transport properties of metallic Shirakawa polyacetylenes with different dopant species, Synth. Met. 69 (1995) 71–72.  H. Masuda, D. Asano, Preparation and properties of polypyrrole, Synth. Met. 135 (2003) 43–44.  A.A. Arrieta Almario, R.L. Tarazona Caceres, Study of kinetic formation and the electrochemical behavior of polypyrrole ﬁlms, J. Chil. Chem. Soc. 54 (2009) 14–19.  R. Ansari Khalkhali, W. Price, G.G. Wallace, Quartz crystal microbalance studies of the effect of solution temperature on the ion-exchange properties of polypyrrole conducting electroactive polymers, React. Funct. Polym. 56 (2003) 141–146.  B. Fabre, J. Simonet, Electroactive polymers containing crown ether or polyether ligands as cation-responsive materials, Coord. Chem. Rev. 178 (1998) 1211–1250.  H. Korri Youssouﬁ, A. Yassar, S. Baiteche, M. Hmyene, F. Garnier, Designing polypyrrole-based sensors: selective electrochemical cation in aza crown ethers, Synth. Met. 67 (1994) 251–254.  V.M. Schmidt, J. Heitbaum, Ion exchange mechanism of polypyrrole and poly-Nmethylpyrrole with toslylate as doping anion: an electrochemical quartz crystal microbalance study, Electrochim. Acta 38 (1993) 349–356.  F. Beck, P. Braun, M. Oberst, Organic electrochemistry in the solid stateoveroxidation of polypyrrole, Ber. Bunsen. Phys. Chem. 91 (1987) 967–974.  A.G. Rangamani, P.T. McTigue, B. Verity, Slow deactivation of polypyrrole during oxidation–reduction cycles, Synth. Met. 68 (1995) 183–190.  X. Wang, X. Cheng, D. Sun, Interaction in anaerobic biodecolorization of mixed azo dyes of Acid Red 1 and Reactive Black 5 under batch and continuous conditions, Colloids Surf. A: Physicochem. Eng. Aspects 379 (2011) 127–135.  L.-X. Wang, X.-G. Li, Y.-L. Yang, Preparation, properties and applications of polypyrroles, React. Funct. Polym. 47 (2001) 125–139.  A.S. Liu, M.C. Bezerra, L.Y. Cho, Electrodeposition of polypyrrole ﬁlms on aluminum surfaces from a p-toluene sulfonic acid medium, Mater. Res. 12 (2009) 503–507.  G. Zhang, F. Yang, M. Gao, X. Fang, L. Liu, Electro-Fenton degradation of azo dye using polypyrrole/anthraquinonedisulphonate composite ﬁlm modiﬁed graphite cathode in acidic aqueous solutions, Electrochim. Acta 53 (2008) 5155–5161.  M. Li, W. Li, J. Liu, J. Yao, Preparation and characterization of PPy with methyl orange as soft template, J. Mater. Sci.: Mater. Electron. 24 (2013) 906–910.  J. Ferreira, M.J.L. Santos, R. Matos, O.P. Ferreira, A.F. Rubira, E.M. Girotto, Structural and electrochromic study of polypyrrole synthesized with azo and anthraquinone dyes, J. Electroanal. Chem. 591 (2006) 27–32.  J. Lawson, J. Erjavec, Basic two-level factorial experiments, in: Modern Statistics for Engineering and Quality Improvement, Cengage Learning, Duxbury, 2001, pp. 199–241, Chapter 8.  S. Asavapiriyanont, G.K. Chandler, G.A. Gunawardena, D. Pletcher, The electrodeposition of polypyrrole ﬁlms from aqueous solutions, J. Electroanal. Chem. 177 (1984) 229–244.  P. Palanisamy, A. Agalya, P. Sivakumar, Polymer composite—a potential biomaterial for the removal of reactive dye, E-J. Chem. 9 (2012) 1823–1834.  D.A. Kaplin, S. Qutubuddin, Electrochemically synthesized polypyrrole ﬁlms: effects of polymerization potential and electrolyte type, Polymer 36 (1995) 1275–1286.